INVESTIGATION OF THE EFFECT OF CARBON NANOTUBES ON HYBRID GLASS/CARBON FIBER REINFORCED COMPOSITES
Department of Textile Engineering Textile Engineering
ISTANBUL TECHNICAL UNIVERSITY GRADUATE SCHOOL OF SCIENCE ENGINEERING AND TECHNOLOGY
INVESTIGATION OF THE EFFECT OF CARBON NANOTUBES ON HYBRID GLASS/CARBON FIBER REINFORCED COMPOSITES
M.Sc. THESIS Shahrukh SHAHBAZ
Department of Textile Engineering Textile Engineering
Thesis Advisor: Prof. Dr. Ömer Berk BERKALP
ISTANBUL TECHNICAL UNIVERSITY GRADUATE SCHOOL OF SCIENCE ENGINEERING AND TECHNOLOGY
İSTANBUL TEKNİK ÜNİVERSİTESİ FEN BİLİMLERİ ENSTİTÜSÜ
KARBON NANOTÜP KULLANIMININ KARBON/CAM HİBRİT KOMPOZİTLER ÜZERİNDEKİ ETKİSİNİN İNCELENMESİ
YÜKSEK LİSANS TEZİ Shahrukh SHAHBAZ
Tez Danışmanı: Prof. Dr. Ömer Berk BERKALP Tekstil Mühendisliği Bölümü
Jury Members: Prof. Dr. Cevza CANDAN ... Istanbul Technical University
Prof. Dr. Ziya ÖZEK ... Namık Kemal University
Prof. Dr. Ömer Berk BERKALP ... Istanbul Technical University
Shahrukh Shahbaz, a M.Sc. student of ITU Graduate School of science Engineering and Technology student ID 503131814, successfully defended the thesis entitled “INVESTIGATION OF THE EFFECT OF CARBON NANOTUBES ON HYBRID GLASS/CARBON FIBER REINFORCED COMPOSITES”, which he prepared after fulfilling the requirements specified in the associated legislations, before the jury whose signatures are below.
Date of Submission : 02 May 2016
Date of Defense : 27 June 2016
Thesis Advisor: Prof. Dr. Ömer Berk BERKALP ... Istanbul Technical University
To my beloved parents and spouse, Thesis Advisor : Prof. Dr. Omer BERK Berkalp ...
First of all, I would like to thank my advisors, Professor Dr. Ömer Berk BERKALP for their patience, motivation, enthusiasm, immense knowledge aspiring guidance and friendly advice during the thesis work. His guidance helped me in all the time of experimentation and writing of this thesis. I could not have imagined having a better advisor and mentor for my MS thesis and one simply could not wish for a better or friendlier supervisor. I am sincerely grateful to him for sharing his truthful and illuminating views on a number of issues related to the thesis.
Beside my advisor, I would like to thank Professor Dr. Emel ONDER for helping me in using her lab for the dispersion of Carbon Nanotubes by Ultrasonication. I am also thankful to Mr.Erdal and Mr.Osman for their support during Lab activities and Mr. Umut Karaguzel for helping me in mechanical testing. I am also thankful to Mr. Ozcan Dogu KAYA, Derby Conveyor Belts, for giving us a favor to use impact testing machine in his laboratory.
I will use this opportunity to express my gratitude to my parents for supporting me spiritually and through every thick and thin of my life and encouraged me with their best wishes.
I feel immense pleasure to say thanks to BAP ITU who funded for this research project no. 38830 and let us buy the materials and equipment required for our thesis without any difficulty.
Last but not the least, I would like to thank the Department of Textile Engineering, Istanbul Technical University for providing the support and equipment I needed for experimentation and completion of my thesis and the HEC, Pakistan who funded my studies.
xiii TABLE OF CONTENTS
FOREWORD ... xi
TABLE OF CONTENTS ... xiii
ABBREVIATIONS ... xv
LIST OF TABLES ... xvii
LIST OF FIGURES ... xix
SUMMARY ... xxiii
ÖZET ... xxvii
1. INTRODUCTION ... 1
1.1. Purpose of Thesis ... 2
1.2. Literature Review ... 2
1.2.1. Polymer Matrix Composites (PMCS) ... 6
1.2.2. Epoxy resin ... 7
1.2.3. Reinforcement material ... 8
1.2.4. Natural reinforcements ... 9
1.2.5. Synthetic reinforcements ... 9
22.214.171.124. Aramid fibers (Kevlar) ... 9
126.96.36.199. Carbon fiber ... 10
188.8.131.52. Glass fiber ... 10
184.108.40.206. Carbon nanotubes... 12
1.2.6. Hybrid Composite Materials ... 16
1.2.7. Ultrasonication ... 17
1.2.8. Tensile test ... 17
1.2.9. Bending test (Mid Span Loading) ... 18
1.2.10. Impact test (Drop weight test) ... 18
2. EXPERIMENTAL WORK AND METHODOLOGY ... 21
2.1. Safety ... 21
2.2. Preparation of CNT/PAN Dispersion ... 21
2.2.1. Materials and equipment for CNT/PAN dispersion ... 21
220.127.116.11. MWCNTs specifications ... 22
2.2.2. Procedure for CNT/PAN dispersion ... 23
2.3. CNT grafting methodology ... 23
2.3.1. Materials and equipment for CNT grafting ... 23
2.3.2. Procedure for grafting CNTs ... 25
2.4.1. Materials and equipment for preparation of CNT-Epoxy dispersion ... 26
2.4.2. Procedure for CNT-Epoxy dispersion ... 26
2.5. Composite Development ... 27
2.5.1. Materials and equipment for composite development ... 27
2.5.2. Layout of vacuum bagging method ... 29
2.5.3. Procedure for composite development: ... 29
2.6. Tensile Testing ... 31
2.6.1. Materials and equipment for tensile testing ... 31
2.6.2. Specimen preparation for tensile test ... 33
2.6.3. Tensile test procedure ... 34
2.7. Bending Test ... 37
2.7.1. Material and equipment for bending test ... 38
2.7.2. Specimen preparation for bending test ... 38
2.7.3. Bending test procedure... 39
2.8. Impact testing (Drop weight test) ... 41
2.8.1. Specimen preparation for impact testing ... 41
2.8.2. Materials and equipment for impact testing ... 42
2.8.3. Impact testing procedure ... 42
3. RESULTS AND CONCLUSION ... 45
3.1. Tensile testing ... 45
3.1.1. Ultimate tensile strength of CNT grafted composites ... 45
3.1.2. Tensile strength plots for CNT grafted composites ... 46
3.1.3. Tensile strength comparison plots for CNT grafted composites ... 48
3.1.4. Tensile results analysis for CNT grafted composites ... 50
3.1.5. Ultimate tensile strength of CNT-Epoxy dispersed composites ... 51
3.1.6. Stress Strain curves for CNT-Epoxy dispersed composites... 52
3.1.7. Tensile results analysis for CNT-Epoxy dispersed composites ... 54
3.2. Three Point Bending Test ... 57
3.2.1. Bending test results for the CNT grafted composites ... 57
3.2.2. Bending test plots for CNT grafted composites ... 58
3.2.3. Bending strength comparison plots for CNT grafted composites ... 60
3.2.4. Bending test results analysis for CNT grafted composites ... 62
3.2.5. Bending test results for the CNT-Epoxy dispersed composites ... 63
3.2.6. Stress Strain curves for CNT-Epoxy dispersed composites... 64
3.2.7. Bending test results analysis for CNT-Epoxy dispersed composites ... 65
3.3. Impact Strength Test ... 69
3.3.1. Impact strength test results for CNT grafted composites ... 69
3.3.2. Impact strength analysis for CNT grafted composites ... 71
3.3.3. Impact strength test results for CNT-Epoxy dispersed composites ... 72
3.3.4. Impact strength analysis for CNT-Epoxy dispersed composites ... 73
3.4. Suggestions and Practical Application of This Study ... 74
REFERENCES ... 77
CNTs : Carbon Nanotubes PAN : Poly Acrylonitrile
SWCNT : Single walled Carbon Nano Tubes MWCNT : Multi Walled Carbon Nano Tubes CCC : Carbon-Carbon- Carbon
GGG : Glass-Glass-Glass CGC : Carbon-Glass-Glass GCG : Glass-Carbon-Glass DMF : Dimethyl Formamide
xvii LIST OF TABLES
Table 1.1: Mechanical Properties of Different Glass Fibers. ... 12
Table 2.1: Materials and equipment for CNT/PAN dispersion. ... 22
Table 2.2: Materials and equipment for CNT grafting. ... 24
Table 2.3: Material and equipment for CNT-Epoxy dispersion. ... 26
Table 2.4: Materials and equipment for composite development. ... 28
Table 2.5: Table for specimen dimensions for Tensile Strength. ... 34
Table 2.6: Table of specimen dimensions for 3 point bending test. ... 39
Table 3.1: Ultimate tensile strength of CNT grafted composites. ... 45
Table 3.2: Ultimate tensile strength of CNT-Epoxy dispersed composites. ... 51
Table 3.3: Bending (flexural) strength of CNT grafted composites... 57
xix LIST OF FIGURES
Figure 1.1: Vacuum Bagging Set-Up. ... 4
Figure 1.2: Matrix surrounding fibers. ... 6
Figure 1.3: Basic Epoxy Structure. ... 7
Figure 1.4: Synthesis of an epoxide oligomer. ... 8
Figure 1.5: Single Walled CNT and Multiwalled CNT. ... 13
Figure 1.6: SEM image of grown CNTs on carbon fiber (a) a low magnified image of several fibers covered with CNTs, (b) an individual fiber covered with CNTs. ... 14
Figure 1.7: Schematic Illustration for the Formation of MWCNTs-g-PAN Carbon Fiber Precursors. ... 15
Figure 1.8: Schematic reaction of the functionalized MWCNTs with glass fiber coating. ... 16
Figure 2.1: Ultrasonic processor. ... 21
Figure 2.2: CNT dispersion through sonication. ... 23
Figure 2.3: Spray gun. ... 24
Figure 2.4: Clamped reinforcement. ... 24
Figure 2.5: Oven. ... 24
Figure 2.6: Without CNTs and with CNTs glass fabric. ... 25
Figure 2.7: Without CNTs and with CNTs carbon fabric. ... 25
Figure 2.8: Layout for Vacuum Bagging. ... 29
Figure 2.9: Layers of reinforcement covered with mesh flow. ... 30
Figure 2.10: Vacuum check. ... 31
Figure 2.11: CNC machine. ... 32
Figure 2.12: UTM by SHIMADZU. ... 32
Figure 2.13: Extensometer camera. ... 33
Figure 2.14: Test specimen with tabs. ... 33
Figure 2.15: Pictorial representation of tensile test. ... 35
Figure 2.16: Specimen clamped on tensile tester. ... 36
Figure 2.17: Specimen break at maximum load. ... 36
Figure 2.18: 3-point bending test specimen. ... 38
Figure 2.19: Three point bending test. ... 40
Figure 2.20: Midspan loading arrangement. ... 40
Figure 2.21: Loading produced deflection in composite. ... 40
Figure 2.22: Specimen for impact testing. ... 42
Figure 2.23: Drop weight test mechanism. ... 42
Figure 2.24: Drop weight testing equipment. ... 43
Figure 2.25: Impactor falling at the center of the specimen. ... 43
Figure 3.1: Stress-strain curve for [CCC] composites (CNT grafted). ... 46
Figure 3.3: Stress-strain curve for [GCG] composites (CNT grafted). ... 47
Figure 3.4: Stress-strain curve for [GGG] composites (CNT grafted). ... 47
Figure 3.5: [CCC] composites comparison plot for the tensile strength (CNT grafted). ... 48
Figure 3.6: [CGC] composites comparison plot for the tensile strength (CNT grafted). ... 48
Figure 3.7: [GCG] composites comparison plot for the tensile strength (CNT grafted). ... 49
Figure 3.8: [GGG] composites comparison plot for the tensile strength (CNT grafted). ... 49
Figure 3.9: Stress-strain curve for [CCC] composites (CNT-Epoxy Dispersed). .... 52
Figure 3.10: Stress-strain curve for [CGC] composites (CNT-Epoxy Dispersed). .. 52
Figure 3.11: Stress-strain curve for [GCG] composites (CNT-Epoxy Dispersed). .. 53
Figure 3.12: Stress-strain curve for [GGG] composites (CNT-Epoxy Dispersed). .. 53
Figure 3.13: Tensile strength comparison of different technique. ... 54
Figure 3.14: Comparison of stress-strain curve in different techniques for [CCC] composites. ... 55
Figure 3.15: Comparison of stress-strain curve in different techniques for [CGC] composites. ... 55
Figure 3.16: Comparison of stress-strain curve in different techniques for [GCG] composites. ... 56
Figure 3.17: Comparison of stress-strain curve in different techniques for [GGG] composites. ... 56
Figure 3.18: Load vs displacment curve for [CCC] composites (CNT grafted). ... 58
Figure 3.19: Load vs displacment curve for [CGC] composites (CNT grafted). .... 58
Figure 3.20: Load vs displacment curve for [GCG] composites (CNT grafted). ... 59
Figure 3.21: Load vs displacement curve for [GGG] composites (CNT grafted). ... 59
Figure 3.22: [CCC] composites plot for flexural strength (CNT grafted). ... 60
Figure 3.23: [GGG] composites plot for flexural strength (CNT grafted). ... 60
Figure 3.24: [GCG] composites plot for flexural strength (CNT grafted)... 61
Figure 3.25: [CGC] composites plot for flexural strength (CNT grafted). ... 61
Figure 3.26: Load vs displacement curve for [CCC] composites (CNT-Epoxy dispersed). ... 64
Figure 3.27: Load vs displacement curve for [CGC] composites (CNT-Epoxy dispersed). ... 64
Figure 3.28: Load vs displacement curve for [GCG] composites (CNT-Epoxy dispersed). ... 65
Figure 3.29: Load vs displacement curve for [GGG] composites (CNT-Epoxy dispersed). ... 65
Figure 3.30: Flexural strength comparison of different techniques. ... 66
Figure 3.31: Comparison of load vs displacement curves of different techniques for [CCC] composites. ... 67
Figure 3.32: Comparison of load vs displacement curves of different techniques for [CGC] composites. ... 67
Figure 3.33: Comparison of load vs displacement curves of different techniques for [GCG] composites. ... 68
Figure 3.34: Comparison of load vs displacement curves of different techniques for [GGG] composites. ... 68
Figure 3.35: Impact response of [CCC] composites (without CNT, 10 ml, 15 ml, 20 ml, 25 ml) ... 69
Figure 3.36: Impact response of [CGC] composites (without CNT, 10 ml, 15 ml, 20 ml, 25 ml). ... 70 Figure 3.37: Impact response of [GCG] composites (without CNT, 10 ml, 15 ml, 20 ml, 25 ml). ... 70 Figure 3.38: Impact response of [GGG] composites (without CNT, 10 ml, 15 ml, 20 ml, 25 ml). ... 71 Figure 3.39: Impact response of [CCC] composites (without CNT, CNT-Epoxy dispersed). ... 72 Figure 3.40: Impact response of [CGC] composites (without CNT, CNT-Epoxy dispersed). ... 72 Figure 3.41: Impact response of [GCG] composites (without CNT, CNT-Epoxy dispersed). ... 73 Figure 3.42: Impact response of [GGG] composites (without CNT, CNT-Epoxy dispersed). ... 73
INVESTIGATION OF THE EFFECT OF CARBON NANOTUBES ON HYBRID GLASS/CARBON FIBER REINFORCED COMPOSITES
Composites have been attaining great concentration due to the customized properties of reinforcements and matrices and their ability to make high performance materials to replace the current structural materials. The development for the high performance composites with very low weights of materials is keeping high interest levels for the researchers. Few decades later, the discovery of Carbon Nanotubes helped the researchers in making a way for the high performance materials. This discovery also took a positive effect on the performance of composite materials. Carbon Nanotubes have been acknowledged widely for strengthening the mechanical properties of the composites. There are several ways to accommodate the interaction of the CNTs within the composite materials but the costs are high. Chemical Vapour Deposition is an effective way to grow CNTs on reinforcement but it requires higher temperatures and time. The elevated temperature also affects the strength of the reinforcement. The interaction of CNTs with the reinforcement by grafting technique is a suitable technique to induce even distribution of CNTs in the composite materials. According to the study this technique can be used prior to the composite development (i.e. Vacuum bagging, Vacuum Resin Infusion etc.). The temperature requirement is low as compared to the chemical vapour deposition method. The dispersion of CNTs also takes place in an organic solvent which has an advantage over the CNTs dispersion in matrix.
To develop samples of CNTs reinforced composite, flat surface mould is selected. Epoxy resin as matrix material while E-glass fibres and carbon fibres are used as reinforcement material. Three layered composites were prepared with four different combinations. 20 samples were produced, utilizing vacuum bagging technique, of dimension (0.40 x 0.30) 1.2 m2. 16 out of 20 samples are simple composites without grafting of CNTs while others are CNT grafted. Reinforcement is used in the form of woven fabrics. CNTs functionalized with carboxylic group were dispersed in dimethylformamide/PAN suspension through ultra-sonication and sprayed onto the reinforcements in four different volume combinations for each side of the reinforcement i.e. 5 ml, 7.5 ml, 10 ml, 12.5 ml. The process is followed by thermal treatment at 250oC for 3 hours. Reinforcement material is laid on a plain mould after
applying lubricant on the base. Resin was applied through hand layup and composites were manufactured by vacuum bagging technique. Mechanical analysis was carried out. ASTM D-3039 standard procedure was followed for tensile tests while ISO 14125 standard procedure was followed for the bending tests of composite.
Their comparison of the results for the tensile, flexural and impact tests showed interesting improvements in the strength of some composite materials. There was no significant improvement in the tensile properties of the composite materials except for
the [CCC] composites grafted with 15 ml of CNT/PAN. Significant improvement is observed in the flexural properties of the composite materials grafted with CNTs. In order to compare the MWCNTs grafted composites with the Matrix dispersed MWCNTs composites, 4 more specimens were prepared with the same mean quantity of the MWCNTs in CNTs grafted composites. In this case also, the results showed higher raise in the flexural strength up to 70% of the composites but the tensile strength remain unchanged.
The impact strength results also showed valuable information about the usage of the MWCNTs in the composite system. The impact response was improved as the CNT content increased within both the techniques. 15ml – 20 ml of CNT/PAN solution enhanced the impact response to a higher extent whereas the dispersion technique also helped in improving the impact behaviour of the composite material.
This practical study about the effect of carbon nanotubes concludes the influence of techniques by which CNTs are introduced into the composite material and their compatibility with the reinforcement in each technique. The method which is usually carried out to incorporate the CNTs in the composite material is through chemical vapour deposition which consists of very high temperature treatment up to 800 o C. Since this method requires high temperature conditions which is economically not good and the reinforcements can also be degraded when treated with higher temperatures for longer times, the other methods can play an important role in utilizing the maximum performance properties of the reinforcements. Two methods which are used in this study consists of the grafting method and the dispersion method.
Grafting method deals with the interaction of CNTs directly with the reinforcements to incorporate chemical bonds. In order to increase affinity of CNTs towards the reinforcement to produce chemical bonding, the CNTs are functionalized with the acid group (–COOH) prior to the introduction with the reinforcements. Functionalized CNTs and polyacrylonitrile fibres are dispersed in dimethylformamide through ultrasonic processor so that the aggregates could be properly dispersed in the solvent. The dispersion is sprayed on both sides of the reinforcements followed by the oven treatment at 250 oC for 3 hours so that bonding could take place. In this study 4
different volumes of dispersion with same concentration of CNTs were used to observe the effects on mechanical properties of the composite materials. After the oven treatment, composites were manufactured using the hand layup process for resin spreading and excessive resin was extracted out using the vacuum bagging.
The grafting technique was expected to give improved tensile properties to the composites because the direct chemical bonding of CNTs with the reinforcements strengthens the branched networks ultimately empowering the material to hold bigger loads with breaking. The results came out to be good for the [CCC] composites but the degradation was more in other combinations. Further to that the higher volumes of CNT dispersion also drastically degraded the tensile properties of the material which could be the reason of slipping layers over each other. The flexural and impact properties of the materials showed particular improvements in 15ml and 20ml of the spray volumes which was quite significant.
Second methodology which is used in this study for incorporating CNTs in the composite materials is by dispersion method that takes place by dispersing the CNTs in the resin through ultrasonication. The resin dispersed with CNTs is then hand laid up on the reinforcement followed by vacuum bagging to make composites.
Ultrasonic dispersion allowed the CNTs to stack themselves in the matrix in such a way that could produce continuous networking structure which reduces the tendency of micro-cracking in the composites. In the experiments, this methodology showed a little improvements in the tensile direction also but the major improvements were seen in the flexural and impact properties. The impact response of the composite was drastically improved that allowed to absorb more force without cracking.
The usage of glass fabric in hybrid composites also influences the flexural and impact properties of the entire material since it has high flexural properties. Combination of glass fabric along with the CNTs network helps in creating a resultant material with significant improvement in flexural and impact strength properties. The reason lies in the continuous stacking arrangement of the CNTs in the matrix. The stacking arrangement of CNTs depends on the diameter of CNTs which makes it able to acquire more surface area towards the matrix. Smaller diameter nanotubes are considered as fine which allows much closely stacking arrangement causing the continuous network of nanostructures which increases the strength of the composite material.
The alignment of stacking is also considered a very important characteristic. Properties along the axis of the nanotubes are enhanced whereas the properties which are dependent on perpendicular alignment are sacrificed. Proper dispersion of the CNTs in the solvent or resin defines the stacking of nanotubes and reduce the agglomeration of the nanoparticles which cause the deficiency in the strength. The higher quantities of the CNTs in the composite also increases the probability of agglomeration which causes the concentrated stress of very smaller areas which leads to ultimate damage.
KARBON NANOTÜP KULLANIMININ KARBON/CAM HİBRİT KOMPOZİTLER ÜZERİNDEKİ ETKİSİNİN İNCELENMESİ
Kompoziler, takviye elemanı ile reçine özellliklerinin duruma uygun olarak belirlenebilmesi ve bu şekilde mevcut yapı malzemeleri yerini alabilecek yüksek performanslı malzeme yapılabilme kabiliyetleri dolayısıyla, her geçen gün daha da yoğun bir ilgi çekmektedir. Çok düşük ağırlıklarda yüksek performanslı kompozitlerin geliştirilmesi konusu araştırmacıların ilgisini gün geçtikçe arttırmaktadır. Onlarca yıl sonra, Karbon Nanotüplerin (KNT) keşfedilmesiyle birlikte araştırmacıların daha yüksek performanslı kompozit malzemeleri yapabilmeleri de ortaya çıkmıştır. Bu buluş, kompozit malzemlerin performaslarında pozitif bir etki de yaratmıştır. KNT lerin genelde malzemelerin mukavemetinde bir artış sağladığı bilinmektedir. KNT lerin kompozitlere katılması için farklı yöntemler bulunmakla birlikte malzeme maliyetleri ise yüksektir. Bu yöntemlerden Kimyasal Buhar Çökertme yöntemi KNT lerin takviye elemanlarına katılmasında çok etkili olmakla birlikte yüksek sıcaklıklara ve uzun sürelere ihtiyaç vardır. Ayrıca yüksek sıcaklıklara çıkılması takviye elemanının mukavemetine de etki etmektedir.
KNT lerin takviye malzemesine graftlama tekniği ile katılması ise; KNT lerin kompozit malzemelerde düzgün bir şekilde dağıtılması için uygun bir yöntemdir. Çalışmalara göre, bu yöntem kompozitlerin üretiminden önce uygulanmalıdır (diğer deyişle vakumla presleme, vakum reçine infüzyon vb. öncesinde). Aynı zamanda bu yöntemde kimyasal buhar çökertme yöntemine göre sıcaklık da düşük tutulabilir. KNT ler önce bir organic çözücü de disperse edildikleri için KNT lerin doğrudan reçine içinde disperslerine göre de avantaj sağlanmaktadır. Bu sebeplerden dolayı çalışmanın ilk ayağında KNT lerin kompozit malzemeye uygulanmazı için graftlama tekniği seçilmiş ve mazlemeler bu yöntemle üretilmiştir.
KNT takviyeli kompozit üretiminde öncelikle düz bir kalıp seçilmiştir. Reçine olarak epoksi malzemesi, takviye olarak da E-cam ve karbon elyaf kullanılmıştır. Dört farklı kombinasyonda üç katlı lamine kompozit malzemeler üretilmiştir. Çalışma boyunca vakumla kalıplama tekniği ile (0.40 x 0.30) 1.2 m2 boyutlarında 20 adet numune üretilmiş olup bu numunelerden 16 sında graftlama tekniği ile KNT ler takviye elemanına dağıtılmıştır. Takviye elemanı ise dokuma kumaş olarak kullanılmıştır. KNT ler önce ultrasonic karıştırıcı vasıtasıyla dimetilformamid/PAN karışımı içinde çözülmüş ve daha sonra sırasıyla dört farklı konsantrasyon (5 ml, 7.5 ml, 10 ml ve 12.5 ml) ile kumaşların her iki tarafında da spreyle püskürtülmüştür. Kumaşlar önce düz bir kalıbın altına kalıp ayırıcı sürüldükten sonra katmanlar halinde serilmiş ve akabinde elle reçine döküldükten sonra ise vakum kalıplama tekniğiyle kompozit malzeme üretilmiştir. Mekanik analiz olarak da ASTM D-3039 standardına göre kompozitlere mukavemet testi ve ISO 14125 standardına göre ise eğilme testi uygulanmıştır.
Malzemelerin mukavemet, eğilme ve darbe testlerinin sonuçları karşılaştırıldığında bazı kompozit malzeme mukavemetlerinde kayda değer iyileşmeler olduğu görülmüştür. 15 ml KNT/PAN ile graftlanmış olan [CCC] kompozitlerin dışında diğer malzemelerde ciddi bir mukavemet artışı bulunmamaktadır. KNT ile graftlanmış kompozit malzemelerin eğilme özelliklerinde ise kaydadeğer iyileşmeler görülmüştür. Graftlama tekniği sonucunda elde edilen bulgular dahilinde en iyi mekanik etkilerin görüldüğü kompozit malzeme tipi seçilerek, çalışmanın ikinci bir ayağında ise bu tip malzeme üretimi için diğer bir üretim tekniği olarak KNT ler matris içinde dağıtılarak kompozit malzemeye aktarılmıştır. Bu kapsamda; ÇDKNT (çok duvarlı karbon nanotüp) graftlanmış kompozitler ile matris içinde dağıtılmış ÇDKNT kompozitleri kıyaslamak içinde ayrıyeten KNT graftlanmış kompozitlerde kullanılan ÇDKNT miktarı aynı tutularak 4 farklı kompozit malzeme daha üretilmiştir.Bu durumda da, eğilme mukavemetlerinde %70 e varan iyileşmeler görülmüş olup, mukavemet değerleri ise aynı kalmıştır.
Darbe mukavemeti (Serbest ağırlık yöntemi ile-drop weight test) değerleri incelendiğinde ise kompozit malzemelerde ÇDKNT kullanımının etkileri hakkında önemli bulgulara rastlanmıştır. Her iki üretim tekniğiyle (graftlama ve matris içinde dağıtma) üretilen kompozit malzemelerde de KNT uygulamasının artmasıyla darbe mukavemetinin arttığı görülmüştür. 15 ml – 20 ml KNT/PAN solüsyonunun darbe mukavemetini çok arttırdığı görülmekle birlikte matris içinde dağıtma tekniğinin de darbe mukavemetini iyileştirdiği açıkça anlaşılmaktadır.
Karbon nanotüplerin etkileri üzerine yapılan bu pratik çalışmada kompozit malzemeye KNT nin farklı yöntemlerle uygulanması araştırılmıştır. Genelde KNT lerin kompozit malzemeler uygulanması kimyasal buhar çökertmesi ile yapılmakla birlikte, bu yöntemin uygulanması için gerekli olan 800 o C civarı çok yüksek işlem sıcaklığına
ihtiyaç duyulmaktadır. Bu kadar yüksek sıcaklık ekonomik olarak çok verimli olmamakla birlikte, uzun süreli yüksek sıcaklık takviye malzemesine de zarar verebilmektedir. Bu çalışma kapsamında kullanılan iki farklı yöntem olan graftlama ve matris içinde dağıtma yönteminin de kompozit malzemelere KNT ün uygulanması konusunda bir alternatif olacağı da görülmüştür.
Kompozit malzemelerin üretimlerinde -ağırlığı arttırmadan- matris/takviye malzemesinin arayüzey bağlarınının arttırılması ve dolayısıyla malzemenin de mekanik özelliklerinin iyileştirmenin bir alternatifi ise Karbon Nano Tüplerinin kompozit malzeme içine uygulanmasıdır.
Bu çalışmada, Karbon Nano Tüplerin iki farklı yöntemle (graftlama ve matris içinde dağıtma) kompozit malzemelere başarıyla uygulanabildiği görülmüştür.
Karbon Nano Tüp uygulaması, kompozit malzeme üretimlerine fazladan bir maliyet getirmekle birlikte ticari uygulamalarda ürün maliyetini düşürmek maksadıyla – istenildiği takdirde – graftlama yöntemi ile malzemelere kısmi uygulamalarda yapılabilir. Bu şekilde kompozit malzemeye yük gelecek bölgelerin kuvvetlendirilmesi, eğilme mukavemetlerinde arış veya darbe mukavemetinde iyileşmeler sağlanabilir.
Karbon Nano Tüplerin çok farklı tipleri ve ayrıca boyutları bulunmaktadır. Bu çalışma kapsamında sınırlı sürede ve kaynakta belli bir tip ÇDKNT ile çalışma imkanı olmuş
olmakla birlikte, gelecek çalışmalarda farklı tip ve boyutlarda ÇDKNT kullanımı ile çok daha yüksek mekanik özellikler elde etmek mümkün olabilir.
ÇDKNT lerin ayrıca çok iletken malzemeler olduğu bilinmektedir dolayısıyla mekanik etkiler dışında malzemelere elektriksel özellikler de kazandırılabilir. Bu malzemelerin gelecekte elektrik uygulamalarında da önü açık görünmektedir. KNT takviyeli sistemlerin elektriksel özellikleri gelecek dönemlerde özel kompozit malzemelerin üretilmesi için bir imkan olabilir.
Bilhassa düşük ağırlıkta ve fakat yüksek mukavemetli karbon kompozitlerin KNT ile mukavemetin daha da arttırılması uzay ve yapı uygulamaları için yararlı olabilir. Mukavemet artışı dışında eğilme özelliklerinde görülen iyileşmeler de, bu malzemelerin otomotiv sanayinde ve spor malzemeleri sektöründe yer bulabileceğini göstermektedir. Eğilme mukavemetinin bilhassa önemli olduğu kasklar, tamponlar, koruyucu padlar gibi malzemeler için KNT ile takviyelendirilmiş kompozit malzemeler kullanılabilir.
Kompozit malzemelerin hibritleşmesinin farklı etkiler gösterdiği görülmüştür. Hibritleşme için malzemenin kat sayısı ve takviye elemanın farklı yönlerde yerleştirilmesi de önemlidir. Gelecek çalışmalarda bu parametrelerin de arttırılması hibritleşmenin etkilerini daha da iyi ortaya çıkaracaktır.
Bu çalışma neticesinde, son ürün özelliklerine göre takviye malzemesi, matris malzemesi ve karbon nano tüp tipi ile boyutunun birbirine uyumlu ve iyi şekilde seçildiği ve ayrıca uygun bir yöntemle üretim yapıldığı takdirde kompozit malzemelerin mekanik özelliklerinde iyileştirme sağlayabileceği görülmüştür.
1 1. INTRODUCTION
Composite materials are made of at least two different materials. It is superior and unique in performance. Egyptians and Mesopotamian settlers were the first to make use of composites. They used mixture of mud with straws to create strong and durable buildings in 1500 B.C. Mongols developed reinforced bow by the combination of wood, bone and animal glue and then wrapped the bows in birch bark in 1200 A.C. Before the invention of gunpowder these bows were the most powerful weapon on earth. Modern era of composites starts with the invention of plastic in early 1900 that replaced natural glues and resins. Plastics are not strong enough to provide support for structural applications. Reinforcements were needed, that can provide rigidity and strength. In 1935, high performance fibres like glass fibre were developed. Plastic was light and glass fibre was strong; their combination introduced a new trend in material sciences. In 2nd world war alternative light weight but high strength materials were needed for applications like military aircraft industry. Fibre glass composites were also used to shelter the electronic radar systems as they are transparent to radio frequencies. Until the utilization of drop-weight testing machines in 1970’s to estimate the impact strength, the dynamic repose of composites was not focused (Lifshitz, 1976).
After the world war 2nd, composites industry started growing in full swing. The introduction of surf board made of glass fibre composite revolutionized the sports industry. Composites are now involved almost in every sport equipment e.g. bats, rackets, wickets, baskets, sticks etc. In peace days, lower demand of military products, scientist found the application of composites in other fields of life. First commercial composite boat hull was developed in 1946. Brandt Goldsworthy, developed light weight composite surfboard which revolutionized the sports industry. New manufacturing techniques were developed with the passage of time driven by need for alternative materials. In 1970’s the composite industry began to mature. Better resins and advanced reinforcement fibres were developed that found applications in civil, transport, aerospace, agriculture, medical and sports.
For last 30 years composites are the most important industrial materials. Composite industry is still evolving and pushing the limits to acquire advance materials, designs and manufacturing techniques (Abdullah). A detailed study of production and evaluation of properties of Carbon Nanotubes reinforced hybrid composites has been carried out in this project, focusing the effect changing quantities of CNTs in different combinations. For this purpose Vacuum bagging technique is chosen as a processing route for the polymer matrix composites.
Composites have been used in the marine industry since the early 1950’s. Composite vessels feature in almost every area of the marine market, from small leisure craft to large yachts, fishing boats, lifeboats, passenger ferries, pilot boats, floating shopping centre, hulls of catamarans, hovercrafts, sail and surf boards, dry dock caissons and sluice gates. The appearance of composite vessels is aesthetically pleasant and is weather and corrosion resistant, resulting in reduced maintenance compared with other metallic materials. High performance resins are combined with high strength fibres such as glass, carbon and poly aramid to manufacture vessels with outstanding physical properties. Specialised resins impart toughness to conventional polyesters; have enabled the production of high performance craft which can withstand extreme impact and flexural loading without cracking during extreme performance. Developments in other products such as core materials, now allow the manufacture of light weight, stiff, high performance craft that are extremely resistant to the marine environment.
1.1. Purpose of Thesis
The purpose of the this thesis is to manufacture the CNTs reinforced Carbon, Glass and Hybrid composites through grafting technique, and to study the effect of CNTs on the mechanical properties of the composites. Furthermore to investigate the optimal amount of CNTs to get the improved mechanical results in various composites. 1.2. Literature Review
Materials are combined in a way to minimize the effect of their deficiencies in a composite that enable us to make better use of their properties. This process freed the designer of constraints related to the selection of material for a specific use. Different
phased materials are combined to give a product with optimized properties called Composite material. Tougher and lighter materials have made possible to fulfil particular design requirements. Individual components remain separate and distinct in the composite structure (Chapman & Hall, 1998). Composites materials are among the oldest and newest of structural materials. Composites are developed by mixing at least two materials to produce a non-reversible material. They consist a bulk material called Matrix and a reinforcement of some kind and are characterized by high strength, better stiffness, cost, high performance, electrical properties and simple manufacturing techniques (Chapman & Hall, 1998) (Awan, et al., 2009).
Main function of the matrix is to surround the disperse phase i.e. reinforcement. It keeps the fibres together and oriented. It also works as a medium that distribute external load over the fibres to minimize the effect of load. Factors that can affect the mechanical properties of a composite are fibre type, fibre volume fraction, orientation of the fibres and the thickness of the laminate. Mechanical characteristics of constituents with respect to composite are shown in figure 1.1 (Robertson, et al., 1992). After the Iijima’s report about CNTs in 1991, scientists have been taking more interest in the unique atomic structure and properties of CNT’s, such as high aspect ratio, high strength-to-weight ratio, good mechanical properties (their axial tensile strength and elastic modulus were theoretically expected to be as high as 200 GPa and 1–2 TPa (Robertson, et al., 1992), respectively), extraordinary electrical and thermal properties (electric-current-carrying capacity as compared with copper wires is 1000 times higher (Avouris & Collins, 2000), thermally stability retains up to 2800°C in a vacuum or inert atmosphere and thermal conductivity is about twice to that of diamond (Kim, et al., 2001)). These extraordinary properties of CNTs entitles themselves with new scientific and technological opportunities as unique ideal filler material in composites. Composite manufacturing process is a goal oriented process. Each process has its own characteristics that define the type of product to be produced. It allows the composite industry to provide the best solution to the customer need. It involves various operations depending on the availability of technology, provided facilities and personnel skills. The variation in the manufacturing process is also due to vast variety of composite materials and their applications. End use, production volume, size of product, economic targets, labour intensity, materials involved, required skills, surface complexity and appearance, production rate, tools and required equipment are the
factors that are considered while choosing a manufacturing process to produce a composite with desired specification. A consistent product can be achieved by controlling parameters like fibre thickness, resin type, fibre volume fraction and its orientation in the resin. It follows steps to minimize cost, reduce voids and internal stresses (Scott Bader Company Ltd, 2005).
To achieve the manufacturing goals different combination of tools, materials and processing methods are combined to developed manufacturing technique. It is evident that the technique for manufacturing composite is based on the complexity of product and also batch size.
Resin alone is very brittle and its excess can weaken the product. As the vacuum bagging involves hand layup hence the laminate will always begin in oversaturated state and the process still depends on factors like reinforcement, resin type and time. Vacuum bagging utilizes the technique of drawing excess resin out of the reinforcements through vacuum pressure. This technique results in the minimum amount of resin holding the reinforcement and eventually the laminate approach prepreg levels. Figure 1.1 shows the vacuum bagging arrangement and stepwise introduction of resin into reinforcement by vacuum pressure. Vacuum bagging is a little clean process, splashing, spattering and hovering can be avoided. It provides an average working environment. However it is still important to ventilate the work place and follow appropriate safety measures (Ratna, 2009).
Figure 1.1: Vacuum Bagging Set-Up.
95% of the fibres used in reinforced composites are the glass fibres. They are cheap, easy to manufacture and gives high strength and stiffness to the composite. It has lower density with higher resistance to chemicals and good insulation properties but can break easily if prone to prolonged tensile stresses. However it shows good tensile strength if higher stresses are applied in shorter time frames.
Molten glass is drawn into fine threads to produce glass fibres. Freshly drawn glass fibres are protected from contact with hard surface and atmosphere to get undamaged and defect free fibres. Glass fibres are inorganic and strong fibres but lack rigidity due to their molecular structure. S-glass (higher strength glass) has better properties than E-glass in terms of strength and thermal stability but its use is limited due to higher cost (Chiu & Cheng, 2002). Glass fibres are available in short, long and continuous form. The dimension of fibres is characterized by aspect ratio. Longer fibres with smaller diameter add more strength to the composites. Ends of the fibre carry fewer loads with respect to its diameter. Surface imperfections causes fracture in the glass fibre (Starr, 1995).
Bonding at interface between fibre and matrix is important factor in the determination of mechanical properties of fibre reinforced polymers. It is noticed that the adhesion between the resin matrix and fibre is the main precondition for the transfer of load. Laminates are subjected to various predominated stresses on the basis of their end use. The properties and fracture analysis of polyester panels is a complex and demanding field of study. Predominant load is considered as basis for the selection of composite for an application (Bunsell, 1988).
Sandwich structure composites are special category of composite family. They are fabricated by attaching two thin, strong and stiff skins to light weight core material. Separating two materials with a light weight material in between increases the stiffness and strength of the structure at a low weight and cost. It enables light weight construction, freedom of design and low cost alternative to many counterparts (Paolo, et al., 1997).
The quality of the composite and its reproducibility depends on the route of production. Improper fibre to resin ratio, unoriented, broken fibres and non-uniform fibre distribution that results in matrix rich regions, gaps, overlaps or other faults in the arrangement of reinforcement layers, air voids, poorly bonded interlaminar regions, incorrect state of resin cure, resin cracks, transverse ply cracks due to thermal mismatch stresses, localized damage due to mechanical impact around machined holes are the defects may be present in any manufactured composites (Jeong, 1997). Various procedures are standardized to evaluate the defects in any manufactured composite. Standards are used to characterize the properties of the composite.
6 1.2.1. Polymer Matrix Composites (PMCS)
Materials like polyester and epoxy have limited use on their own for structural application because their mechanical properties are not high with respect conventional construction materials like metals. One good aspect of these materials is that they can be easily formed into complex shapes. If reinforced with some strong material can improve mechanical properties. Similarly high performance fibres have high tensile and compressive strength but practically these properties cannot be utilized due to the fact that surface damages are produced when stressed. In order to overcome this problem high strength fibres are combined with resin to produce composite material having optimized properties of all the constituents. By the combination of different resins to reinforcements, composites with good tensile, bending, toughness properties along with good resistance to environmental degradation can be achieved. Figure 1.2 shows the fibres surrounded by matrix in composite structure (Roylance, March 24, 2000).
Figure 1.2: Matrix surrounding fibers.
Polymers possess an important property that they are composed of long chain molecules which has many repeating units. Their use is very common because they infiltrates very easily. According to the response to heat treatment, they can be classified as Thermosets and Thermoplastics.
Thermosets are branched chains polymers. Once cured cannot become liquid again on heating. The resin and hardener or resin and catalyst are mixed, a non-reversible reaction starts giving a hard infusible product with 3D bonded network of polymer chains. Phenolic resins produce volatile by products while others don’t. Above glass transition temperature the mechanical properties depletes because thermosets become flexible. Due to lower viscosity they infiltrate very easily and contribute to the strength and stiffness of the product. Thermosets show good resistance to chemicals. They are
brittle laminates with limited high temperature sustainability especially in hot-wet conditions. Thermosets wets the reinforcement more easily than thermoplastics (Pickering, 2006).
1.2.2. Epoxy resin
Epoxies are being used in order to bind the strengthening fibre and locking them in a position so that they can sustain their position to do their job. Fibres are placed in specific directions in the fibre reinforced structures to focus the reinforcement according to need and the epoxy helps in retaining the position of fibers where they are needed. The aim of the epoxy matrix is to surround the fiber and transfer the loads to the fibers even though it is a strong material itself. It helps in protecting the fibers from damage and offers impact resistance (Christine, n.d.).
Thermosetting polymer resins in which the resin molecule contains one or more epoxide groups are known as Epoxies. The chemistry can be customized by the molecular weight or viscosity as required by the end use to make it a perfect option. Two main types of epoxies (figure 1.3), glycidyl epoxy and non-glycidyl are available. Glycidyl epoxy resins can be briefly defined as either glycidyl-amine, glycidyl-ester, or glycidyl-ether. Non-gylcidyl epoxy resins are either cycloaliphatic or aliphatic resins.
Figure 1.3: Basic Epoxy Structure.
One of the most common glycidyl epoxy resins is manufactured by using Bisphenol-A, and is synthesized in a reaction with epicholrohydrin as shown in figure 1.4 ( Fink, 2013). The other commonly used type of epoxy is novolac based epoxy resin. These resins have a thermosetting nature and they have a requirement of suitable hardener to let them cure.
Figure 1.4: Synthesis of an epoxide oligomer.
Epoxy resins require a curing agent for the setting up which is commonly called a hardener. Usually amine based curing agent are used generally. In polyester or vinyl ester resins the resin is catalysed with a small (up to 3%) addition of a catalyst, whereas epoxy resins usually require the addition of the curing agent at a much higher ratio of resin to hardener.
Although being very resistant cured epoxy degrades on exposure to UV. The surface attains a chalky appearance and loses strength. A UV protection layer can be beneficial in this respect. At elevated temperatures Epoxy loses strength.
Epoxies have influenced a wide range of applications such as fiber-reinforced plastic materials, general purpose adhesives and strong chemically resistant coatings and finishes.
1.2.3. Reinforcement material
Reinforcement adds mechanical properties to the composites. Primary function of reinforcement is to carry load along the direction of their orientation. Mechanical properties of the fibre, its surface interaction with resin, orientation and fibre volume fraction are the factors that define the contribution of reinforcement in composites and most of its properties. For higher end use synthetic reinforcements are used but natural reinforcements are also for many applications (Taranu, 2008). Carbon Nanotubes are also proven to be a source of extraordinary value addition to the reinforcements, such
as Glass and Carbon, as they share the high tensile properties to the resultant reinforcement.
1.2.4. Natural reinforcements
Natural fibres, Asbestos (Mineral Fibres), Cellulose (Vegetal Fibre), Collagen and Silk (Animal Fibre) are used as reinforcement for many application. Natural fibres are cheaper source of reinforcement but have lesser mechanical properties than manmade fibre (Taranu, 2008). Wood Plastic Composites (WPCs) have acquired a wide range of applications in construction and building sector, usually as lumber for railing and decking systems. They also have an advantage of higher stiffness than thermoplastics and are equipped with a natural “wood” look (Mohd Ishak & Taib, 2015).
Changing trends in the world and sustainability issues have forced the manufacturers to use more environment friendly materials such as biodegradable composites. The preparation of the biodegradable composites involves combining of biodegradable polymers with natural fibres (Mohd Ishak & Taib, 2015). Polylactic acid (PLA) can be served as biodegradable polymer and kenaf fibre (KF) as in natural fibre or filler. For sustainable economic development, bamboo industry has been mentioned as an effective source for bio composite fibres, which offers minimal production cost and can bring a revolution in the world of supply chain and manufacturing (Abdul Khalil, et al., 2015).
Synthetic fibre-reinforced composites having good physical properties with high performance at low weight can be substituted by jute-reinforced thermoplastic laminates and composites. Jute fibre composites have sufficient potential to influence the automobile industry, the footwear industry, construction, furniture, and the toy sectors (Khan & Khan, 2015).
1.2.5. Synthetic reinforcements 18.104.22.168. Aramid fibers (Kevlar)
Aramid fibres are man-made organic fibres based on aromatic polyamide chains. DuPont developed aramid fibres. They are closely related to nylon. Aramids have low solubility due to aromatic groups they cannot be drawn so are spun from liquid crystalline solution. They have pale yellow color with high strength and low density hence gives very high specific strength. Aramids have fair compressive strength i.e.
1/8th of its tensile strength because of anisotropic structure. They have good impact resistance with elongation to fracture value (3.5-4%) in Kevlar 29 and Compressive strength of aramid fibres is similar to E-Glass. In longitudinal direction it is very difficult to stretch the aramid fibre because of its structure but in other directions the planes are loosely attached. They show good resistance to abrasion, chemical and thermal degradation. Prolong exposure to UV light can cause degradation to Aramid fibres (Chatzi & Koenig, 1987).
22.214.171.124. Carbon fiber
Polyacrylonitrile (PAN) based fibres having unusual properties of graphite and is obtained by controlled pyrolysis of an organic fibre “PAN” precursor in 4 steps (Transformation, stabilization, carbonization and graphitization). Its Degree of molecular chains alignment depends on processing route and Planes are oriented along the fibre axis. Its main feature is alignment of graphite sheets along fibre direction. Commercial Carbon fibre is normally sized with low molecular weight epoxies to avoid defects due to rubbing among fibres, easy handling and improve bonding with resin. Carbon fibres show anisotropic behaviour and its mechanical properties depend on amount of graphite and basal planes. Strength of carbon fibre depends on percentage of defects. (Inclusion voids). It has good thermal and electrical properties and negative CTE in fibre direction (Department of defense, USA, 23 Jan 1997). 126.96.36.199. Glass fiber
Glass Fibre is SiO2 based amorphous fibre. It contains 50-60% of SiO2 with host of
other metal oxides. Its raw material is cheap but the processing route is not sophisticated. It is the backbone of Information Technology Sector. The properties of Glass Fibre can be tailored by altering its chemical composition. They show isotropic behaviour. Glass fibres have high strength but stiffness. Mechanical properties decay above 400-500oC and ultimately melts. Glass fibres corrode in alkaline environment
and are not resistant to water especially sea water but are not expensive with respect to counterparts (Chapman & Hall, 1998) (Department of defense, USA, 23 Jan 1997). S-Glass has high tensile strength and modulus with better wet strength retention than E-Glass and is used in aerospace and ballistic armour. Its composition is 65% SiO2,
melted form through electrically heated platinum bushes. Commercial glass fibre is normally sized with low molecular weight epoxies to avoid defects due to rubbing among fibres, chemical attack, easy handling and improve bonding with resin (Kinsella, et al.).
The Glass should be smooth with no gaps among the strands to get the best surface finish. It is better to use number of layers of lower weight glass instead the heavy and bulky one to fit the contours of the part. The bridging in the corner causes resin race tracking and leads to poor fill. The glass is laid try into the mould. Different methods are used to keep the glass in place especially on vertical surfaces. It can be achieved by using adhesive backed glass or by using adhesive sprays to standard glass fabric. The adhesives are specially developed for resin infusion process. Limitation of Glass fibre is less tolerance to prolonged loading temperature and moisture. Its disadvantage is further pronounced by the fact that the brittleness leads to a catastrophic failure without any prior warning. Mechanical properties of different Glass fibre types are listed in table 1.1 (Lund, 2010).
The initial application of the glass fiber was to protect radar equipment. It was also used as ducting in airplane engine nacelles. The first usage of the fiberglass in the main airframe construction was in Spitfire in England but it didn’t come out into production. In 1953 Chevrolet put their first production of their model Corvette in which the body was composed of fiberglass composite. Fiberglass bodies significantly reduce the weight of the machine but their commercial production hasn’t yet succeeded the metallic industry. Instead they are particularly famous for replacement body parts, custom and kit auto markets. The tooling costs are also low as compared with metal press assemblies.
Table 1.1: Mechanical Properties of Different Glass Fibers.
A-glass C-glass D-glass E-glass ECR-glass AR-glass R-glass S-2-glass Density (g/cubic cm) 244 2.52 2.11-2.14 2.58 2.72 2.7 2.54 2.46 Tensile Strength (Mpa) at 196oC 5380 5310 5310 8275 Tensile Strength (Mpa) at 23oC 3310 3310 2415 3445 3445 3241 4135 4890 Tensile Strength (Mpa) at 371oC 2620 2165 2930 4445 Tensile Strength (Mpa) at 538oC 1725 1725 2140 2415 Modulus of Elasticity (GPa) at 23oC 68.9 68.9 51.7 72.3 80.3 73.1 85.3 86.9 Modulus of Elasticity (GPa) at 538oC 81.3 81.3 88.9 Elongation % 4.8 4.8 4.6 4.8 4.8 4.4 4.8 5.7 188.8.131.52. Carbon nanotubes
CNTs have proven to be the ultimate strongest known material which makes the discovery of CNT a benchmark in nanotechnology (Iijima, 1991). CNTs are actually hollow cylinders of carbon atoms. They have an appearance of rolled tubes of graphite, and their walls have hexagonal carbon rings. Two types of nanotubes are there: single-walled nanotubes (SWNTs) and multisingle-walled nanotubes (MWNTs), which can be
differed by the arrangement of graphene cylinders (Ganesh, March 2013). Figure 1.5 represent SWCNTs and MWCNTs structures.
Figure 1.5: Single Walled CNT and Multiwalled CNT.
The composites can be more effectively reinforced by CNTs as compared to conventional fibres as they share extraordinary large interfacial contact area with the matrix but with very less weight penalty. Scientists have observed that addition of only 1% of CNTs by weight in a matrix material can result in the increase in stiffness of the composite film by 36–42% and the tensile strength by 25% (Qian, et al., 2000). Apart from using independently CNTs can be used in combination with other common reinforcements like poly-acrylonitrile fibres, carbon fibres and glass fibres for improving, mechanical, electrical and thermal properties of the composites (Fernándeza, et al., 2013) (Wang & Qiu, 2010).
There are a few problems associated with the use of CNTs which include the preparation of structure controlled CNTs retaining the high purity and consistency leading to high performance and the breaking up of bundled CNTs to uniformly disperse and distribute them within a polymer matrix. One more issue is improvement of load transfer from matrix to CNT reinforcement (Du, et al., 2007).
For Carbon Fabric there have been a lot of studies which are focused on achieving an effective method for CNT/CF hybridization. The results can be summarized in two categories: the direct growth method of CNTs on the CF surface by chemical vapour deposition (CVD) (Kim, et al., 2013) and the spray coating of CNTs on the CF surface (He, et al., 2007) or electrophoresis (Bekyarova, et al., 2007).
It has been observed that the CNT growth technique can achieve much higher concentrations of CNTs in a composite as compared to that of dispersion in the matrix. This technique also avoids common problems with CNTs like agglomeration, filtration
and increased viscosity which puts some hurdles in determining the actual CNT contents (Romanov, et al., 2015). Figure 1.6 shows the CNT growth on carbon fiber through SEM image.
Figure 1.6: SEM image of grown CNTs on carbon fiber (a) a low magnified image of several fibers covered with CNTs, (b) an individual fiber covered with CNTs. The main problem reported with the CVD-based method is that it requires high-temperature process over 700 C and layers of ceramic buffers to prevent the deactivation of catalysts (Kim, et al., 2012). In addition to that the mechanical properties of CFs are also degraded after the CVD process (Kim, et al., 2013).
Multiwall carbon nanotubes (MWCNTs) are usually preferred over single wall carbon nanotubes (SWCNTs) due to their lower cost, easier production and better dispersion (Sharma & Lakkad, 2015).
Volkan Eskizeybek, Ahmet Avcı & Ahmet Gülce in 2015 reported a decrease of 11% in ultimate tensile strength of glass fabric/CNT/epoxy multi scale composite whereas toughness was increased up to 57% (Eskizeybek, et al., August, 2015). Geunsung Lee, Kwang Duk Ko Young Chang Yu, Jinyong Lee, Woong-Ryeol Yu, Ji Ho Youk in 2015 observed a 22% enhancement in the tensile strength of the CNT/PAN grafted carbon epoxy composite as compared with the pristine CF composite (Lee, et al., 2015). The CNT grafting process through spray coating can be a helpful tool to ensure high mechanical properties in a localized area of a composite material.
Eslam Soliman, Usama Kandil and Mahmoud Reda Taha observed a significant improvement in the flexural strength, modulus and toughness of the off-axis specimens of epoxy nanocomposites reinforced with carbon woven fabric. The addition of 1.5 wt. % of COOH-MWCNTs in epoxy resulted in the average increase of 28% and 19% in flexure strength and flexure modulus respectively (Soliman, et al., 2014).
The grafting of CNTs on the reinforcements is particularly being used for the hybridization of carbon fabrics. MWCNTs functionalized with carboxylic group can be grafted onto the fabric body in order to improve the properties of the reinforcement. Mohammad M. Fares, Fahmi A. Abu Al-Rub, and Khansa’a H. Massadeh produced MWCNTs-g-carbon precursors by using COOH functionalized MWCNTs with PAN which increased the thermal stability up to 850oC and also improved the UV absorption (Fares, et al., 2015). The step by step formation of MWCNTs-g-PAN carbon fibre precursor can be seen from figure 1.7.
Figure 1.7: Schematic Illustration for the Formation of MWCNTs-g-PAN Carbon Fiber Precursors.
The interaction of MWCNTs with the glass fibre coating was investigated by the researchers to know the possible chemical bonding between the two entities. Fibre coating plays a significant role on the deposition of MWCNTs onto glass fibres and their bonding. The chemical analysis of the glass fibres and its coating indicates the presence of multiple reactive functional groups such as carbonyl, hydroxyl, and epoxy groups that can react with the carboxyl and hydroxyl functional groups MWCNTs as shown in figure 1.8 (Ku-Herrera, et al., 2015).
Figure 1.8: Schematic reaction of the functionalized MWCNTs with glass fiber coating.
Proper dispersion followed with adequate interfacial adhesion is required in order to make CNTs as an effective reinforcement in polymer composites (Ma, et al., 2010). 1.2.6. Hybrid Composite Materials
Hybrid composite laminates are those comprising of multiple type of reinforcement materials. These composite materials facilitates the customization of the reinforcement properties by using different types of reinforcements. Carbon and glass fibres have a wide range of application which demands high strength, low weight and low cost. The reinforcements used to make a hybrid material help in improving certain properties, e.g., the glass fibres has a lower modulus with higher strain-to-failure in comparison to carbon fibres. In this case the flexural strength of carbon fibre-reinforced polymer (CFRP) composites can be significantly improved by substituting some of the carbon fibre laminas by glass fibre ( Kalantari, et al., 2015).
The resultant composite manufactured by carbon and glass fibre hybridization not only influences the flexural strength and stiffness but other key properties also such as cost and weight. Subsequently the glass fibres are heavier and cheaper than carbon fibres, hybridization of a CFRP composite through the incorporation of glass fibres leads to a lower material cost but higher density. The weight and cost reduction are the two major concerns that leads in the designing process of hybrid composite structures ( Kalantari, et al., 2015).
The length of fibre, fibre orientation, and fibre shape and fibre material of the reinforcements are the few influential factors that affect the performance of the composite’s mechanical performance.
17 1.2.7. Ultrasonication
It can be explained as the process of applying ultrasound energy to agitate nanoparticles in a solution for desired purposes. An ultrasonic bath or an ultrasonic probe is used as Sonicator. This technique is based on the principle that attenuated waves are induced in the liquid molecules when ultrasound propagates through a series of compression. These vibrations tend to overcome the interactions between the CNTs which results in the dispersion.
The sonication treatment provides the ability to the surfactant molecules to be adsorbed onto CNT surface by overcoming the interactions produced by the hydrophobic, electrostatic and van der Waals forces (Yu, et al., 2012). Firstly the liquid is adsorbed on the CNT surface which reduce the size of big bundles to smaller bundles. After sufficient time the solution contains individual CNTs and tiny bundles of CNTs. The main parameters of the sonication process are time and power. The power of the sonication system should be optimal because lower powers cannot separate the CNT bundles and the higher power could create more than required shear stress on CNTs resulting in their damage.
The power is more important characteristic of the sonication system as compared with the sonication time (Yu, et al., 2012).
1.2.8. Tensile test
The concept of tensile test can be explained through normal stress and shear stress. A specimen or sample is gripped at both ends and is pulled apart. The amount of stress in the specimen can be found by calculating the force applied by the grips over the cross sectional area normal to the applied force. The ultimate tensile strength is the highest value of force that the tester measures for a specimen while modulus of elasticity is found as the slope of the line presenting stress as the function of strain (Hermann & Locke , November 2006).
The international standard for tensile testing is given by ASTM and its designation is “D 3039/D 3039M – 00 “. It determines the in plane tensile properties of Polymer matrix composites reinforced by high modulus fibres. Thin flat strip with rectangular cross section is mounted on a mechanical testing machine and a monotonic load is applied in tension while the load is being recorded. The ultimate strength of material
is the maximum load carried before failure. ASTM D- 3039 basically determines the in plane properties of high modulus fibre reinforced polymer composites. The reinforcement forms are limited to continuous or discontinuous fibres while the test specimen of polymer composite is symmetric with respect to test direction (ASTM D 3039/D3039M – 00, , 2002).
When a material is subjected to a load, the force distributes itself through the material in the form of internal stresses. The behaviour of material during failure is determined by the amount of stress that exists inside it. Mathematically, Stress is Force applied over the area normal to the applied force while shear stress is the force applied parallel to the area. Stress is expressed in Pascal (Pa). Material under stress deforms either by stretching, contracting or bending. This resulting deformation is called strain and can be defined as change of length of specimen divided by the total length of specimen. Strain is a dimensionless quantity (Askeland, 1990).
1.2.9. Bending test (Mid Span Loading)
It determines the properties of sandwich constructions that are subjected to flat wise flexure. Load is applied is applied in a manner to produce curvature of the sandwich facing planes. Flexural stiffness, core shear strength and shear modulus or the facing compressive and tensile strengths of sandwich construction can be evaluated. For this purpose ISO standard 14125 is followed. Sandwich stiffness and core shear modulus can be evaluated by calculating deflection of sandwich flexural specimens. ISO 14125 allows the use of either single (midspan) loading or two-point loading. These are generally called three-point and four-point flexure testing, respectively. The configuration of flexure can be altered to perform both the tests. In order to perform three points loading test, one loading head is removed while the remaining one apply load at the centre of the specimen (Standard test method for flexural properties of sandwich constructions. ).
1.2.10. Impact test (Drop weight test)
This test methodology is used to determine the damage resistance of composites facing a drop-weight impact event (ASTM International). ASTM D7136 test standard was used to carry this test. This test is carried by a fall of a mass with a semispherical tip from a certain height onto the laminate. The weight of the impactor was 35 kg. This
test was not carried for the standardized specifications since ASTM D7136 specifies a value of 5.50 kg for the impactor, but allows the use of other values. The energy with which the impactor strikes the test specimen is dependent on the mass of impactor and the height from which it is dropped (Justo, et al., 2015).
The area of the damage and the indentation depth helps in measuring the impact resistance of the specimen.